Trivalent Cation-Controlled Phase Space of New U(IV) Fluorides, Na3MU6F30 (M = Al(3+), Ga(3+), Ti(3+), V(3+), Cr(3+), Fe(3+)): Mild Hydrothermal Synthesis Including an in Situ Reduction Step, Structures, Optical, and Magnetic Properties.
Yeon, Jeongho; Smith, Mark D.; Morrison, Gregory; Zur Loye, Hans-Conrad; Inorganic chemistry 54 (2015) 2058–2066; doi:10.1021/ic503034t

data_4342339
_publ_section_title
;
 Trivalent Cation-Controlled Phase Space of New U(IV) Fluorides, Na3MU6F30
 (M = Al(3+), Ga(3+), Ti(3+), V(3+), Cr(3+), Fe(3+)): Mild Hydrothermal
 Synthesis Including an in Situ Reduction Step, Structures, Optical, and
 Magnetic Properties.
;
_journal_issue                   4
_journal_name_full               'Inorganic chemistry'
_journal_page_first              2058
_journal_page_last               2066
_journal_paper_doi               10.1021/ic503034t
_journal_volume                  54
_journal_year                    2015
_chemical_formula_moiety         'Al F30 Na3 U6'
_chemical_formula_sum            'Al F30 Na3 U6'
_chemical_formula_weight         2094.13
_chemical_name_systematic
; 
 ? 
;
_space_group_crystal_system      trigonal
_space_group_IT_number           165
_space_group_name_Hall           '-P 3 2"c'
_space_group_name_H-M_alt        'P -3 c 1'
_symmetry_space_group_name_Hall  '-P 3 2"c'
_symmetry_space_group_name_H-M   'P -3 c 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   9.771(3)
_cell_length_b                   9.771(3)
_cell_length_c                   12.896(7)
_cell_measurement_reflns_used    7317
_cell_measurement_temperature    567(2)
_cell_measurement_theta_max      28.4533
_cell_measurement_theta_min      2.4068
_cell_volume                     1066.3(7)
_computing_cell_refinement       'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_data_collection       'SMART Version 5.631 (Bruker, 2001)'
_computing_data_reduction        'SAINT-Plus Version 6.45 (Bruker, 2001)'
_computing_molecular_graphics    various
_computing_publication_material  various
_computing_structure_refinement  'SHELXL-2013 (Sheldrick, 2013)'
_computing_structure_solution    'SHELXS97 (Sheldrick, 1997)'
_diffrn_ambient_temperature      567(2)
_diffrn_measured_fraction_theta_full 0.993
_diffrn_measured_fraction_theta_max 0.993
_diffrn_measurement_device_type  'Bruker SMART APEX CCD diffractometer'
_diffrn_measurement_method       'omega and phi scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0436
_diffrn_reflns_av_sigmaI/netI    0.0152
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            12940
_diffrn_reflns_theta_full        28.35
_diffrn_reflns_theta_max         28.35
_diffrn_reflns_theta_min         2.41
_exptl_absorpt_coefficient_mu    45.750
_exptl_absorpt_correction_T_max  0.2619
_exptl_absorpt_correction_T_min  0.1209
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS Version 2.05 (Bruker, 2001)'
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    6.522
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       'hexagonal plate'
_exptl_crystal_F_000             1736
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.04
_exptl_crystal_size_min          0.04
_refine_diff_density_max         0.978
_refine_diff_density_min         -1.390
_refine_diff_density_rms         0.251
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.217
_refine_ls_matrix_type           full
_refine_ls_number_parameters     62
_refine_ls_number_reflns         899
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.217
_refine_ls_R_factor_all          0.0205
_refine_ls_R_factor_gt           0.0188
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0130P)^2^+10.9563P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0403
_refine_ls_wR_factor_ref         0.0410
_reflns_number_gt                862
_reflns_number_total             899
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ic503034t_si_002.cif
_cod_data_source_block           Na3AlU6F30
_cod_depositor_comments
'Adding full bibliography for 4342339--4342344.cif.'
_cod_database_code               4342339